View metadata, citation and similar papers at core.ac.uk brought to you by CORE
provided by National Tsing Hua University Institutional Repository IEEE ELECTRON DEVICE LETTERS, VOL. 24, NO. 4, APRIL 2003 209 GaAs MOSFET With Oxide Gate Dielectric Grown by Atomic Layer Deposition P. D. Ye, G. D. Wilk, J. Kwo, B. Yang, H.-J. L. Gossmann, M. Frei, S. N. G. Chu, J. P. Mannaerts, M. Sergent, M. Hong, K. K. Ng, and J. Bude
Abstract—For the first time, a III-V compound semiconductor MOSFET with the gate dielectric grown by atomic layer deposition (ALD) is demonstrated. The novel application of the ALD process on III-V compound semiconductors affords tremendous function- ality and opportunity by enabling the formation of high-quality gate oxides and passivation layers on III-V compound semicon- ductor devices. A 0.65- m gate-length depletion-mode n-channel # GaAs MOSFET with an AlPOQ gate oxide thickness of 160 e shows R P a gate leakage current density less than 10 A/cm and a max- imum transconductance of 130 mS/mm, with negligible drain cur- rent drift and hysteresis. A short-circuit current-gain cut-off fre- quency of 14.0 GHz and a maximum oscillation frequency mx of 25.2 GHz have been achieved from a 0.65- m gate-length device. Index Terms—Atomic layer deposition, depletion mode, GaAs MOSFET. Fig. 1. Two-terminal gate s– characteristics of an Al O aGaAs MOSFET. Source and drain are grounded together. Inset: Schematic view of a NTRODUCTION I. I depletion-mode n-channel GaAs MOSFET with ALD-grown Al O as gate MOS integrated-circuit technology dominates the dielectric. C Si-based microelectronics industry. The key for the aggressive yet successful scaling of Si CMOS technology is deposition of Ga O and Ga O Gd O dielectric films on the outstanding material properties of SiO and the SiO /Si the GaAs surface in an ultrahigh-vacuum multichamber molec- interface. The benefits of a GaAs-based MOSFET are well ular beam epitaxy (MBE) system has been shown to provide known, based on the success of Si technology. This motiva- a high-quality interface with a low –. Promising tion has attracted great interest for decades –. Gallium results have been demonstrated in both inversion-channel arsenide (GaAs)-based devices potentially have great advan- and depletion-mode GaAs MOSFETs using this technique tages over silicon (Si)-based devices for both high-speed and –. high-power applications, in part from an electron mobility In this letter, we report for the first time a MOSFET on a III-V in GaAs that is 5 greater than that in Si, and from the substrate with an Al O gate dielectric deposited by atomic availability of semi-insulating GaAs substrates. In contrast to layer deposition (ALD). Al O is a highly desirable gate di- GaAs MESFETs and HEMTs, both of which exhibit a severe electric from both a physical and electrical characteristics stand- limitation on forward gate bias of a few tenths of a volt (arising point: Al O has a high bandgap 9eV, a high breakdown from the nature of Schottky barrier heights), GaAs MOSFETs field (5–10 MV/cm), and high thermal stability (up to at least feature a much larger logic swing, which provides much greater 1000 C) and remains amorphous under typical processing con- flexibility in digital IC design. ditions. Furthermore, Al O is easily wet-etched yet is robust The main obstacle to GaAs-based MOSFET devices is the against interfacial reactions and moisture absorption (i.e., non- lack of high-quality, thermodynamically stable insulators on hygroscopic). The Al O gate oxide is grown by ALD, which GaAs that can match the device criteria as SiO on Si, e.g., a is a variant of CVD, and has recently shown promise for use in mid-bandgap interface-trap density of 10 cm -eV. high-k gate dielectrics for Si CMOS . ALD is an ex situ, Many approaches – have been applied to grow a gate robust manufacturing process that is already commonly used oxide on GaAs, such as thermal, anodic, and plasma methods throughout the Si industry. This process does not require ul- or direct deposition of thermodynamically stable oxide films trahigh-vacuum conditions for wafer transfer between semicon- on GaAs. These approaches have had limited success, however, ductor epi-layer growth and oxide layer deposition and may find due to a high and unacceptable value. Recently, in situ wide applications in microelectronics manufacturing.
II. DEVICE STRUCTURE AND PROCESS Manuscript received December 19, 2002; revised February 19, 2003. The re- view of this letter was arranged by Editor D. Ritter. The device structure of the fabricated depletion-mode The authors are with Agere Systems, Murray Hill, NJ 07974 USA (e-mail: [email protected]). n-channel Al O /GaAs MOSFET is shown in the inset of Digital Object Identifier 10.1109/LED.2003.812144 Fig. 1. A 1500- undoped GaAs buffer layer and a 700-
0741-3106/03$17.00 © 2003 IEEE 210 IEEE ELECTRON DEVICE LETTERS, VOL. 24, NO. 4, APRIL 2003
Fig. 2. Drain current versus drain bias in both forward (dashed black line) and reverse (solid gray line) sweep directions as a function of gate bias. The s– characteristics show negligible hysteresis in drain current.
Si-doped GaAs layer (4 10 /cm ) were sequentially grown by MBE on a (100)-oriented semi-insulating 2-in GaAs sub- strate. After the semiconductor epilayer growth, the wafer was transferred ex situ to an ASM Pulsar2000™ ALD module. A 160- -thick Al O oxide layer was deposited at a substrate temperature of 300 C, using alternately pulsed chemical precursors of Al CH (the Al precursor) and H O (the (b) oxygen precursor) in a carrier N gas flow. Each precursor Fig. 3. (a) Drain current versus gate bias in both forward (dashed black line) undergoes a self-limiting reaction at the surface, and the Al O and reverse (solid gray line) sweep directions. Dotted line is transconductance film is thereby grown with excellent thickness and uniformity versus gate bias at aQV. (b) Peak transconductance g versus frequency from dc to several gigahertz. The g is essentially constant for frequencies precision. A post-deposition anneal was done at 600 C for above 20 Hz, indicating that efficient charge modulation of the channel can be 60 s in an oxygen ambient. Device isolation was achieved by achieved over the entire useful frequency range of the device. oxygen implantation. Activation annealing was performed at 450 C in a helium gas ambient. Using a wet etch in diluted HF, We ascribe the asymmetric gate – characteristics to different the oxide on the source and drain regions was removed while carrier transport mechanisms and barrier heights in the different the gate area was protected by photoresist. Ohmic contacts bias polarities. The current is larger when the semiconductor is were formed by e-beam deposition of Au/Ge/Au/Ni/Au and biased to inject electrons compared with when the metal is bi- a lift-off process, followed by a 425 C anneal in a nitrogen ased to inject electrons. ambient. Finally, conventional Ti/Au metals were e-beam The DC – characteristics of a MOSFET show a clean pin- evaporated, followed by liftoff to form the gate electrodes. The choff at a gate voltage of 2.5 V (see Fig. 2) with a gate length source-to-gate and the drain-to-gate spacings are 0.75 m. of 1 m and gate width of 100 m. Device operation is achieved The sheet resistance and contact resistance is 1.3 k sq. and for positive bias voltages, and no substantial – hysteresis 1.5 mm. The gate lengths of the measured devices are is observed in the drain current drift in both the forward and re- 0.65, 0.85, 1, 2, and 4 m. The process requires four levels of verse sweep directions. This indicates that no significant mobile lithography (alignment, isolation, ohmic, and gate), all done bulk oxide charge is present and that density of slow interface using a contact printer. traps is low. The small and values for V are mainly limited by the surface mobility of the GaAs layer and/or III. ELECTRICAL RESULTS AND DISCUSSIONS higher near the conduction-band edge. In order to separate Fig. 1 demonstrates the low gate leakage of these devices in these two factors, more detailed capacitance and Hall measure- the gate – characteristics of a MOSFET with an Al O gate ments as a function of gate bias are underway. Ongoing exper- oxide thickness of 160 . The gate length and width of the de- iments with an inserted In Ga As channel show significant vice are 0.65 m and 100 m, respectively. For gate operation improvement in both and performance for V, between a bias ( )of 4Vto 4 V, the gate leakage current is which can be attributed to the higher surface mobility of the less than 100 pA, corresponding to 10 A/cm . Based on the In Ga As layer. data in Fig. 1, these MOSFET devices clearly exhibit extremely Fig. 3(a) illustrates the drain current as a function of gate bias low gate leakage currents over a 14-V gate bias range, which is in both the forward and reverse sweep directions in the satura- more than three orders of magnitude lower than for MESFETs tion region. The device shows negligible hysteresis. The slope of under similar bias. The forward breakdown voltage is 8 V for the drain current shows that the peak extrinsic transconductance a 160- -thick Al O layer, which corresponds to a breakdown of the 1- m gate length device is 100 mS/mm. The peak electric field larger than 5 MV/cm. This verifies the high quality can be improved from 90 mS/mm at a 4- m gate length of the ALD-grown oxide even after the full transistor process. to 130 mS/mm at 0.65- m gate length. Fig. 3(b) shows the YE et al.: GaAs MOSFET WITH OXIDE GATE DIELECTRIC GROWN BY ATOMIC LAYER DEPOSITION 211
negligible – hysteresis and a gate leakage current density less than 10 A/cm . The stability under stress indicates that the ALD-grown Al O film and the Al O /GaAs interface are of high quality. These results provide new opportunities to explore many other alternative dielectrics for use as gate oxides and as effective passivation layers on III-V compound semiconductor devices.
REFERENCES  T. Mimura and M. Fukuta, “Status of the GaAs metal-oxide-semicon- ductor technology,” IEEE Trans. Electron Devices, vol. ED-27, pp. 1147–1155, 1980.  C. W. Wilmsen, Ed., Physics and Chemistry of sss– Compound Semi- conductor Interfaces. New York: Plenum.  M. Hong, C. T. Liu, H. Reese, and J. Kwo, “Semiconductor-insulator interfaces,” in Encyclopedia of Electrical and Electronics Engineering, J. G. Webster, Ed. New York: Wiley, vol. 19, pp. 87–100.  S. Tiwari, S. L. Wright, and J. Batey, “Unpinned GaAs MOS capacitors and transistors,” IEEE Electron Device Lett., vol. 9, pp. 488–490, Sept. Fig. 4. RF characteristics of Al O /GaAs MOSFETs with gate length and 1988. width of 0.65 and 100 "m, respectively. RF tester includes two identical devices  C. L. Chen, F. W. Smith, B. J. Clifton, L. J. Mahoney, M. J. Manfra, and with total gate length of 200 "m. Inset: f and f for different gate lengths. A. R. Calawa, “High-Power-Density GaAs MISFETs with a low-tem- The dashed line illustrates f a v aP%v . perature-grown epitaxial layer as the insulator,” IEEE Electron Device Lett., vol. 12, pp. 306–308, June 1991.  Y. H. Jeong, K. H. Choi, and S. K. Jo, “Sulfide treated GaAs MISFETs peak as a function of frequency, measured from dc to sev- with gate insulator of photo-CVD grown P N film,” IEEE Electron eral gigahertz, under typical operating conditions ( V, Device Lett., vol. 15, pp. 251–253, May 1994. V). It can be seen that the remains essentially  E. I. Chen, N. Holonyak, and S. A. Maranowski, “Al Ga As–GaAs metal-oxide semiconductor field effect transistors formed by lateral constant for frequencies above 20 Hz, indicating that efficient water vapor oxidation of AlAs,” Appl. Phys. Lett., vol. 66, pp. charge modulation in the channel can be achieved over the en- 2688–2690, 1995. tire useful frequency range of the device. Furthermore, note that  J. Y.Wu, H. H. Wang, Y.H. Wang, and M. P. Houng, “A GaAs MOSFET with a liquid phase oxidized gate,” IEEE Electron Device Lett., vol. 20, there is about a 20% decrease in from 20 Hz down to dc. A pp. 18–20, Jan. 1999. model calculation of this change in gives an upper limit for  T. Waho and F. Yanagawa, “A GaAs MISFET using an MBE-grown of 5 10 to 10 cm -eV. CaF gate insulator layer,” IEEE Electron Device Lett., vol. 9, pp. 548–549, Oct. 1988. From S-parameter measurements, the short-circuit cur-  G. W. Pickrell et al., “Improvement of wet-oxidized Al Ga As @x $ rent-gain cut-off frequency and the maximum oscillation IA through the use of AlAs/GaAs digital alloys,” Appl. Phys. Lett., vol. frequency are determined by biasing the devices 76, pp. 2544–2546, 2000.  J. C. Ferrer, Z. Liliental-Weber, H. Reese, Y. J. Chiu, and E. Hu, at V and V. Under these conditions, “Improvement of the interface quality during thermal oxidation of the 0.65- m gate length device shows GHz and Al Ga As layers due to the presence of low-temperature-grown GHz. These values are obtained by extrapolating GaAs,” Appl. Phys. Lett., vol. 77, pp. 205–207, 2000.  S. Yokoyama, K. Yukitomo, M. Hirose, Y. Osaka, A. Fischer, and K. the short-circuit current gain and the unilateral power Ploog, “GaAs MOS structures with Al O grown by molecular beam gain (U) curves, respectively, using 20 dB/decade slopes, as reaction,” Surf. Sci., vol. 86, pp. 835–840, 1979. shown in Fig. 4. The inset of Fig. 4 illustrates the and  J. Reed, G. B. Gao, A. Bochkarev, and H. Morkoc, “Si N /Si/Ge/GaAs metal-insulator-semiconductor structures grown by in situ chemical as a function of gate length. As the trend shows, and vapor deposition,” J. Appl. Phys., vol. 75, pp. 1826–1828, 1994. can be significantly improved by reducing the gate length. The  M. Hong, M. Passlack, J. P. Mannaerts, J. Kwo, S. N. G. Chu, N. Moriya, observed versus gate length is quite close to the theoretical S. Y. Hou, and V. J. Fratello, “Low interface state density oxide-GaAs structures fabricated by in situ molecular beam epitaxy,” J. Vac. Sci. relation of , where is 6 cm/s. Technol. B, vol. 14, pp. 2297–2300, 1996. The long-term drain-current drift behavior of the  M. Passlack et al., “Low h , thermodynamically stable Ga O –GaAs Al O /GaAs MOSFET is also studied when the devices interfaces: Fabrication, characterization, and modeling,” IEEE Trans. Electron Devices, vol. 44, pp. 214–225, Feb. 1997. are biased at a stress condition of V and V.  M. Hong et al., “Epitaxial cubic Gadolinium oxide as a dielectric for The long-term drain-current drift is less than 3% for a stress Gallium Arsenide passivation,” Science, vol. 283, pp. 1897–1900, 1999. @ A @ A H ` period of 12 h. The result is comparable with the best data  J. Kwo et al., “Passivation of GaAs using Ga O Gd O , x`IXH films,” Appl. Phys. Lett., vol. 75, pp. 1116–1118, 1999. reported previously , indicating that the ALD-grown Al O  F. Ren et al., “Demonstration of enhancement-mode p- and n-channel film and Al O /GaAs interface are of very high quality. GaAs MOSFETs with Ga O @Gd O A as gate oxide,” Solid-State Elec- tron., vol. 41, pp. 1751–1753, 1997.  Y. C. Wang et al., “Demonstration of submicron depletion-mode GaAs IV. CONCLUSIONS MOSFETs with negligible drain current drift and hysteresis,” IEEE Electron Device Lett., vol. 20, pp. 457–459, Sept. 1999. We have demonstrated the first ALD-grown insulated gate  M. Passlack et al., “Self-aligned GaAs p-channel enhancement mode MOSFET on III-V substrates, using Al O gate dielectric MOS heterostructure field-effect transistor,” IEEE Electron Device Lett., for n-channel depletion-mode GaAs devices. The 0.65- m vol. 23, pp. 508–510, Sept. 2002.  G. D. Wilk, R. M. Wallace, and J. M. Anthony, “High-k gate dielectrics: gate-length device exhibits an extrinsic transconductance of Current status and materials properties considerations,” J. Appl. Phys., 130 mS/mm, an of 14 GHz, and an of 25 GHz, with vol. 89, pp. 5243–5275, 2001.